- Email: [email protected]

Contents lists available at ScienceDirect

Automation in Construction j o u r n a l h o m e p a g e : w w w. e l s ev i e r. c o m / l o c a t e / a u t c o n

The use of artiﬁcial neural networks in adiabatic curves modeling Gregor Trtnik a,b, Franci Kavčič b, Goran Turk a,⁎ a b

University of Ljubljana, Faculty of Civil and Geodetic Engineering, Jamova 2, SI-1115 Ljubljana, Slovenia I GM AT d.d. Building Materials Institute, Polje 351c, Ljubljana, Slovenia

A R T I C L E

I N F O

Article history: Accepted 7 April 2008 Keywords: Fresh concrete Adiabatic hydration curves Experiments Artiﬁcial neural network

A B S T R A C T Adiabatic hydration curves are the most suitable data for temperature calculations in concrete hardening structures. However, it is very difﬁcult to predict the adiabatic hydration curve of an arbitrary concrete mixture. The idea of modeling adiabatic temperature rise during concrete hydration with the use of artiﬁcial neural networks was introduced in order to describe the adiabatic hydration of an arbitrary concrete mixture, depending on factors which inﬂuence the hydration process of cement in concrete. The inﬂuence of these factors was determined by our own experiments. A comparison between experimentally determined adiabatic curves and adiabatic curves, evaluated by proposed numerical model shows that artiﬁcial neural networks can be used to predict adiabatic hydration curves effectively. This model can be easily incorporated in the computer programs for prediction of the thermal ﬁelds in young concrete structures, implemented in the ﬁnite element or ﬁnite difference codes. New adiabatic hydration curves with some other initial parameters of the concrete mixture can be easily included in this model in order to expand the range of suitability of artiﬁcial neural networks to predict the adiabatic hydration curves. © 2008 Elsevier B.V. All rights reserved.

1. Introduction Concrete is the most commonly used structural material and is composed of individual base materials. Every base material has some inﬂuence on the hydration process of cement in concrete. Of course, cement has the greatest inﬂuence being one of the base materials, which is the foundation for hydration process. Hydration is an exotermic reaction during which heat liberates. Increased temperature of mixture caused by heat generation during hydration accelerates the hydration process. Development of the hydration heat is one of the most important processes worth observing during setting and hardening of concrete in particular during concreting of large volumes [1]. During hardening of concrete there arise high thermal gradients near the surface of the concrete block as a result of relatively low thermal conductivity. Extensive development of heat of hydration during concreting in summer period may lead to overheating of concrete. Hydration process of cement in concrete in laboratory conditions is usually the basis for further prediction of behavior of concrete in structures. Development of hydration reactions and processes in qualitative respect may be followed with the aid of monitoring the development of hydration heat by direct and indirect calorimetric methods. Adiabatic heat measurements are the most convenient for producing continuous heat of hydration curves under curing condition close to or almost identical with mass curing [2]. Adiabatic hydration ⁎ Corresponding author. Tel.: +386 1 4768 614; fax: +386 1 4768 629. E-mail address: [email protected] (G. Turk). 0926-5805/$ – see front matter © 2008 Elsevier B.V. All rights reserved. doi:10.1016/j.autcon.2008.04.001

curves would be the most suitable starting point for temperature calculations in hardening structures. Therefore, the adiabatic curves are judged to be of great practical importance. It is well known [2–4], that kinetics and intensity of the hydration process is affected by many factors, such as environmental temperature and moisture content, cement composition, ﬁneness of grinding, water–cement ratio, type of cement, initial temperature of fresh concrete mix, presence of additives and admixtures etc. There exist numerous empirical equations to predict the adiabatic curves, i.e. the adiabatic temperature rise T(t) of concrete mixture. Morabito [5] for example used the following empirical relationship T ðt Þ ¼

t ; n þ mt

ð1Þ

where m and n are constants to be determined empirically for each kind of concrete mixture. Kavčič [4] used the equation T ðt Þ ¼ Tl exp ðmt n Þ;

ð2Þ

where T∞ [°C] is the temperature at the end of the hydration process. Ammar et al. [6] give the following equation d c T ðt Þ ¼ a þ b exp ; t

ð3Þ

where a, b, c and d are constants to be determined for each kind of concrete mixture. Eqs. (2) and (3) are both mathematical functions that produce a curve having “S” shape with exactly one inﬂection point.

G. Trtnik et al. / Automation in Construction 18 (2008) 10–15

The main disadvantage of these equations is that the empirical coefﬁcients have to be determined experimentally and speciﬁcally for each concrete mix. This is time-consuming and hence expensive. Particularly in the design stage of the project, when the designer wants to evaluate the effects of changes in the concrete mix on the temperature and strength development, it would be of great advantage if these input adiabatic curves could be generated with the use of adequate numerical models. Therefore, the successful development of a general formula to predict the adiabatic hydration curve for an arbitrary concrete would be a great advantage. Some numerical programs exist which are able to predict the adiabatic hydration curves for an arbitrary concrete mixture [2,7]. In the Van Breugel model [2], the degree of hydration (and corresponding adiabatic hydration curve) is modeled as a function of the particle size distribution and chemical composition of cement, w/c ratio and reaction temperature. The cement particles are modeled as digitized spheres, randomly distributed in a three dimensional body and the hydrating cement grains are simulated as growing spheres. As cement hydrates, the cement grains gradually dissolve and a porous shell of the hydration products is formed around the grains. This result in an outward growth or expansion of the particles. These hydrates ﬁrst cause the formation of small isolated clusters. Big clusters are formed, when small cement particles become embedded in the outer shell of other particles, which promotes the outward growth of these particles. As a hydration progresses, the growing particles become more and more connected and the material changes from the state of a suspension to the state of a porous solid. In the NIST model [7], the cement particles are represented as a collection of elements (pixels). The model operates on three dimensional images of multi-phase cement particles generated to match speciﬁc characteristic of two-dimensional SEM images of real cements. Hydration of cement was simulated by applying a cellular-automata algorithm for dissolution, diffusion, and reaction of the four major cement phases, C3S, C2S, C3A and C4AF. Evsukoff et al. [8] presented a data mining approach for modeling the adiabatic temperature rise during concrete hydration. The objective of this study is to check the ability of the artiﬁcial neural networks (ANNs) to predict the adiabatic hydration curve of an arbitrary concrete mixture depending on some parameters, which inﬂuence the hydration process of cement in concrete. Therefore, the necessary data on the inﬂuence of these factors on the adiabatic temperature rise were gathered and analyzed by our own experiments.

11

2. Experimental work 2.1. Test equipment and procedure To achieve the objective of this study, adiabatic calorimeter of Building Materials Institute IGMAT, which uses air as the coupling media, was used. A ventilator at the top of the chamber guarantees a good circulation of air in the chamber. Adiabatic calorimeter is shown in Fig. 1. The temperature of the concrete in adiabatic calorimeter during the test was measured automatically. Adiabatic calorimeter was connected to the PC and a suitable PC software was prepared for this purpose (see Fig. 1). The temperature was read every 10 min, and the duration of one test was about 168 h (one week). This means that about 1000 data were saved for each concrete mixture. Within this study, as many as 22 adiabatic tests were performed. These adiabatic curves are well distributed over the predetermined ranges parameter's values. The inﬂuence of type of cement, amount of cement, w/c ratio, initial temperature of fresh concrete and the inﬂuence of some chemical and mineral admixtures on the hydration process of cement in concrete were investigated. Table 1 lists the different parameter values for each mixture. 2.2. Experimental results Fig. 2a shows all 22 adiabatic hydration curves, which were used in this study. The inﬂuence of initial concrete temperature, type of cement, and amount of cement on the hydration process can be seen from Fig. 2b, c, and d, respectively. It can be seen from Fig. 2b that the higher initial temperature of the fresh concrete results in a more rapid hydration process at the very beginning. Interestingly, it ﬁnally results in a lower temperature increase at the end of the test. This is a well known phenomenon, which was also observed by some other researchers, for example [2,4]. Fig. 2c presents the inﬂuence of the type of cement on the hydration process. Four types of cements, used in Slovenia, were used for this purpose. The most intensive hydration process was observed, when cement type CEM II/A-S, 42.5 R (PCS 30) was used. Fig. 2d shows the inﬂuence of the amount of cement on the hydration process. It is clear that the higher cement content leads to more rapid hydration process.

Fig. 1. Adiabatic calorimeter of Building Materials Institute IGMAT.

12

G. Trtnik et al. / Automation in Construction 18 (2008) 10–15

Table 1 Characteristics of the 22 adiabatic curves Label

Initial 1 [°C]

Cement type

Am. of cement [kg/m3]

Admixture [%]

w/c

A1 A2 A4 SA 30 C1B2 30 PCS 30 PC 30 SA 20 208 2 208 3 208 4 208 5 208 6 208 7 208 8 208 9 ZB 002 ZB 004 ZB 005 ZB 103 ZB 105 ZB 107

20 25 27 22.9 25.3 19.9 26.5 23 18.7 21.3 20.7 12.6 7.2 23.8 24.9 26.2 17.37 13.08 7.89 18.49 12.85 7.94

1 1 1 1 2 3 4 1 3 3 3 3 3 3 3 3 3 3 3 3 3 3

180 180 180 380 350 350 350 280 360 360 360 330 360 360 360 360 370 370 370 370 370 370

0 0 0 0 0 0 0 0 0 0 2 2 2 0 0 0 0 0 0 3 3 3

0.7 0.7 0.7 0.42 0.43 0.45 0.45 0.65 0.5 0.5 0.47 0.45 0.47 0.5 0.5 0.5 0.54 0.54 0.54 0.5 0.5 0.5

For a detailed description of these phenomenons reference is made to the literature [3,4].

activation function intensiﬁes or weakens the signal which is transmitted to other neurons. There are many applications of ANN in structural engineering. Recently, there have been reports on the use of ANN in the modelling the concrete strength, for example [9–11], but lately neural networks have also been efﬁciently used for the prediction of concrete compressive strength based on various non-destructive tests [12– 14]. Graham et al. presented a neural network approach for modeling the ready mix concrete delivery system [15]. The multi-layer feed-forward neural networks are usually employed as the approximators of an unknown functional relation [16]. The geometry of a multi-layer feed-forward neural network is shown in Fig. 3. The input units, which represent the input data, are connected to the ﬁrst layer of hidden units, which are further connected to the units of the next hidden layer. The units of the last hidden layer are connected to the output units, which represent the output data. Each unit is represented by its value yki . Each connection between the units is characterized by its weight wkij. The index i corresponds to the unit number of kth layer, while index j corresponds to the unit number of the (k− 1)th layer. The value of a unit is multiplied by the corresponding weight and added to the value of the signal in the unit of the next layer. In addition, the value of bias neuron or threshold ϑki is added to the equation Xn k1 ð4Þ wkij yk1 þ #ki ; yki ¼ f j j¼1 which is illustrated in Fig. 3. Activation function f(.), which is usually the sigmoid function

3. Artiﬁcial neural networks (ANN) ANNs are networks consisting of an arbitrary number of very simple elements called neurons. Neurons in ANNs are, similarly to the neurons in human brains, interconnected. The connections are deﬁned by weights. Through connections a neuron receives signal from other neurons. The

f ð yÞ ¼

1 ; 1 þ expðyÞ

ð5Þ

enables the modelling of an arbitrary continuous non-linear relation between input and output variables.

Fig. 2. Inﬂuence of the parameters on the adiabatic temperature rise.

G. Trtnik et al. / Automation in Construction 18 (2008) 10–15

13

corresponding to the ﬁve inﬂuencing factors (see Table 1) and the time t, thirty in each hidden layer and one in the output layer corresponding to the adiabatic temperature rise T. The neurons of successive layers are fully connected. The batch of data has been divided into two sets, one for the ANN learning called a learning set and the other for testing the ANN called a testing set. Two studies were done in order to establish the ability of ANN to predict adiabatic hydration curves of arbitrary concrete. Within the ﬁrst study, concrete mixtures with the same cement type were taken into account, while within the second study, all data were used (see the following sections). 5. Teaching and testing the network 5.1. Study 1: Data for cement type 3 Most of the concrete mixtures were prepared with cement type 3, which is one of the most frequently used type of cement in Slovenia. Therefore, in this study twelve curves, labeled PCS 30, 208 2, 208 3, 208 4, 208 8, 208 9, ZB 002, ZB 004, ZB 005, ZB 103, ZB 105 and ZB 107 (see Table 1) were used for teaching the ANN and curve 208 7 was used for testing. Within this study, the cement type was the same for all concrete mixtures, so the number of input neurons was reduced to ﬁve. In this case, none of the input parameters of curve 208 7 had extreme value with respect to parameter values of all other curves analyzed here. We stopped the learning process when the iterations

Fig. 3. Multi-layer feed-forward artiﬁcial neural network.

The set of known input and output values is termed an input– output pair. All pairs are divided into two sets. The ﬁrst one is termed as the learning or training set (about 75% of all data), which is used to determine the connection weights wkij and thresholds ϑki . When the learning procedure ends, meaning that the neural network performs adequately for all input–output pairs in the learning set, the performance of the neural network is assessed on the testing data. In some cases the training procedure becomes ill-conditioned if the input and/or output data are not normalized (see e.g. [17]). Therefore, for numerical reasons, the values of the input and output data have to be normalized. The normalization of the values of output units depends on the range of the activation function f. The training procedure is in fact a general optimization problem in which the minimum of error Ep is sought Ep ¼

2 1 Xn0 Tpi ynpil ; i¼1 2

ð6Þ

nl are the values of neurons in where tpi are the target output values, ypi the output layer nl, i.e. the output values evaluated by ANN, n0 is the number of neurons in the output layer, i.e. the number of output variables. This problem is numerically very demanding since a large number of local minima usually exist. There are two essentially different approaches: error back-propagation (BP) algorithms (which are basically a gradient method) and genetic algorithms (which are in fact a stochastic search).

4. Construction of ANN model A typical MFNN has three or more layers: the input layer, one or more hidden layers and the output layer. While learning, the neural network store the non-linear information between the inﬂuencing factors and the adiabatic temperature rise T in the weight matrix in a dynamic and parallel way, and the network can give the corresponding output upon the input factors while recalling. As the problem was deﬁned as a nonlinear input–output relation between the inﬂuencing factors and the adiabatic temperature rise T, this led us to choose, for our ANN, the 6-3030-30-1 architecture. Therefore, there are six neurons in the input layer,

Fig. 4. Comparison between actual and calculated values of relative temperature.

14

G. Trtnik et al. / Automation in Construction 18 (2008) 10–15

reached 1000, and the grand total learning error (see Eq. (6)) was 0.025. Fig. 4a is an expression of the learning results, each point standing for a learning vector. The nearer the points gather around the diagonal, the better are the learning results. Thus, the learning errors of the points on the diagonal are zero. It can be seen from this ﬁgure, that the 5-30-30-30-1 ANN predicted the testing values with a high accuracy. The coefﬁcient of correlation was R2 = 0.9995 in this case, while the root mean square error (RMSE), deﬁned by vﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ u N u1 X 2 Te;ANN Te;exp RMSE ¼ t N e¼1

ð7Þ

was 0.2006. In Eq. (7) N is a number of all testing data, Te,ANN is the value of temperature rise at time te, evaluated by the ANN model and Te,exp is the value of temperature rise at time te, determined by experiment. Fig. 4b presents the testing adiabatic curve 208 7, which was obtained by experiments (dashed line) and the same curve, obtained by ANN (solid curve). In this case ANN model attain very good prediction accuracy. 5.2. Study 2: All data In this study all data were used for teaching the ANN, except curve 208 3 which was used for testing. At ﬁrst, the curve 208 2 was

Fig. 6. Inﬂuence of the initial temperature on the adiabatic temperature rise with ANN model.

eliminated from the learning set, so the initial temperature Tinit of concrete 208 3 was the lowest among all other initial temperatures of the concretes with the same remaining four input parameters (208 7, 208 8, 208 9) as in the case of concrete 208 3 (see Table 1). The coefﬁcient of correlation between actual and calculated values was R2 = 0.9969 and the RMSE was 0.5115. Fig. 5a shows the correlation between actual and calculated values in this case. Next, the curve 208 2 was included in the learning set, so the initial temperature Tinit was not the lowest any more. The coefﬁcient of correlation between actual and calculated values was R2 = 0.9989 in this case and the RMSE value was 0.3358. Fig. 5b shows the correlation between actual and calculated values in this case. Therefore the accuracy of prediction was better than in the case when the curve 208 2 was not included in the learning set. This indicates that ANN has good capability of interpolation but is not as efﬁcient in the case of extrapolation. 5.3. Use of the ANN model — Example

Fig. 5. Comparison between actual and calculated values of relative temperature. a) Without 208 2, b) with 208 2.

When the learning and testing procedure were ﬁnished and all the weights wkij were established, the programme was installed within Matlab programming environment. The weights from the 2nd study were used for this purpose. The adequateness of the proposed model can be observed from Fig. 6, where the inﬂuence of the initial temperature of fresh concrete mixture is shown. The well known phenomenon, which was explained in Section 2, is observed again. The higher initial temperature leads to the more rapid hydration process at the very beginning and ﬁnally results to the lower temperature increase at the end of the test. It can also be seen from Fig. 6, that a small deviation in the initial temperature Tinit leads to an important and well observed change in the adiabatic hydration curves. Therefore, we conclude the proposed ANN model was quite sensitive. The initial temperatures of the dashed, dotted and solid curves were 22 °C, 22.5 °C and 23 °C, respectively and the other initial parameters were as follows: cement type 3, amount of cement 350 kg/m3, w/c ratio 0.47 and amount of admixtures 0. The computer programs, which are used for prediction of the thermal ﬁelds and thermal cracking in young concrete are usually implemented in the ﬁnite element or ﬁnite difference codes. One of the main inputs in such analysis is the adiabatic temperature rise curve. Unfortunately, it is often time-consuming and difﬁcult to determine the corresponding adiabatic hydration curve. The presented numerical model can be easily incorporated in such computer program and the adiabatic hydration curve can be determined only by entering a variable data set corresponding to the binder physical and chemical properties and concrete mixture proportions.

G. Trtnik et al. / Automation in Construction 18 (2008) 10–15

6. Conclusions The ANN-based model was developed for predicting the adiabatic temperature rise curve of different concrete mixtures. This way, a very good agreement of calculated adiabatic hydration curves and adiabatic hydration curves, obtained by our experiments in suitable adiabatic calorimeter was achieved. It was shown that the learning data are very important and meaningful for the accurate prediction of adiabatic hydration curves. These data have to be selected properly and have to be well distributed over the predetermined ranges of variability. New adiabatic hydration curves with some other initial parameters of the concrete mixture can be easily included in the learning set in order to expand the range of suitability of ANN to predict the adiabatic hydration curves. The presented ANN model of adiabatic curves can be easily incorporated in computer programs, based on ﬁnite element or ﬁnite difference method, which are used for prediction of thermal ﬁelds and thermal cracking in young concrete. Proposed model attains a good prediction accuracy. Some effects of concrete initial parameters (for example the initial temperature of fresh concrete) on adiabatic temperature rise are in good accordance with the well known rules of mix proportioning and other initial characteristics of fresh concrete mixture. Consequently, the application of ANN models to predict the adiabatic hydration curves of concrete is practical and has a prospect of application in construction practice. Notations The following notations are used in the paper ANN artiﬁcial neural network T adiabatic temperature rise [°C] t time a, b, c, d, m, n empirical constants T∞ temperature at the end of the hydration process yki output of neuron i in layer k yjk − 1 output of neuron j in layer k − 1 wkij connection between neuron i in layer k and neuron j in previous layer ϑki threshold value nk number of layers f(.) activation function Ep error between target temperature value Tpi and predicted temperature value ypinl n0 number of all neurons in output layer

nl Tinit RMSE N Te,ANN Te,exp

15

lth output layer initial temperature of concrete root mean square error number of all testing data value of temperature rise at time te, evaluated by the ANN model value of temperature rise at time t e, determined by experiment

References [1] J. Zach, H. Kminova, O. Horky, J. Brozovsky, Determination of intensity of hydration heat development of silicate binders, Proc. The 8th International Conference of the Slovenian Society for Non-Destructive Testing, Application of Contemporary NonDestructive Testing in Engineering, Portorož, Slovenia, 2005, pp. 375–382. [2] K. van Breugel, Simulation of Hydration and Formation of Structure in Hardening Cement-Based Materials — HYMOSTRUC, Ph.D. Thesis, Second Edition, Delft University of Technology, 1997. [3] G. Trtnik, The inﬂuence of chemical admixtures on cold weather concreting (in Slovenian), B.Sc. Thesis, University of Ljubljana, 2004. [4] F. Kavčič, Hydration process of cement in concrete at the adiabatic conditions (in Slovenian), M.Sc. Thesis, University of Ljubljana, 2000. [5] P. Morabito, Apparent Activation Energy, An Example of Determination from Adiabatic Hydration Tests, IPACS Report BE96-3843/2001:19-2, Lulea, Sweden, 2001. [6] C. Ammar, P. Dutron, H. Motteu, J. Dubois, La progression des betons et des mortiers par basses temperatures, C.S.T.C.-C.R.I.C.-SECO, Bruxelles, 1973. [7] D.P. Bentz, CEMHYD3D: A Three-dimensional Cement Hydration and Microstructure Development Modelling Package. Version 3.0, NISRTIR 7232, U.S. Department of Commerce Technology Administration, Gaithersburg, Maryland, 2005. [8] A.G. Evsukoff, E.M.R. Fairbairn, E.F. Faria, M.M. Silvoso, R.D.T. Filho, Modeling adiabatic temperature rise during concrete hydration: a data mining approach, Computers and Structures 84 (31–32) (2006) 2351–2362. [9] S.C. Lee, Prediction of concrete strength using artiﬁcial neural networks, Engineering Structures 25 (7) (2003) 849–857. [10] H.G. Ni, J.Z. Wang, Prediction of compressive strength of concrete by neural networks, Cement and Concrete Research 30 (8) (2000) 1245–1250. [11] S. Lai, M. Serra, Concrete strength prediction by means of neural network, Construction and Building Materials 11 (2) (1997) 93–98. [12] J. Hola, K. Schabowicz, Application of artiﬁcial neural networks to determine concrete compressive strength based on non-destructive tests, Journal of Civil Engineering and Management, 11 (1) (2005) 23–32. [13] M.A. Kewalramani, R. Gupta, Concrete compressive strength prediction using ultrasonic pulse velocity through artiﬁcial neural networks, Automation in Construction 15 (3) (2006) 374–379. [14] J. Hola, K. Schabowicz, New technique of nondestructive assessment of concrete strength using artiﬁcial intelligence, NDT&E International 38 (4) (2005) 251–259. [15] L.D. Graham, D.R. Forbes, S.D. Smith, Modeling the ready mix concrete delivery system with neural networks, Automation in Construction 15 (5) (2006) 656–663. [16] T. Ambrožič, G. Turk, Prediction of subsidence due to underground mining by artiﬁcial neural networks, Computers and Geosciences 29 (5) (2003) 627–637. [17] W.S. Sarle, Neural network FAQ. Periodic posting to the Usenet newsgroup compai.neuralnets. URL: ftp://ftp.sas.com/pub/neural/FAQ.html; 10.07.2007.

Copyright © 2021 COEK.INFO. All rights reserved.